of the three methods of heat transfer – conduction (they are mostly composed of insulating gas) and convection (the microstructure prevents net gas movement). They are good conductive insulators because they are composed almost entirely of gases, which are very poor heat conductors. (Silica aerogel is an especially good insulator because silica is also a poor conductor of heat; a metallic or carbon aerogel, on the other hand, would be less effective.) They are good convective inhibitors because air cannot circulate through the lattice. Aerogels are poor radiative insulators because infrared radiation (which transfers heat) passes through them. Owing to its hygroscopic nature, aerogel feels dry and acts as a strong desiccant. People handling aerogel for extended periods should wear gloves to prevent the appearance of dry brittle spots on their skin. The slight colour it does have is due to Rayleigh scattering of the shorter wavelengths of visible light by the nano-sized dendritic structure. This causes it to appear smoky blue against dark backgrounds and yellowish against bright backgrounds. Aerogels by themselves are hydrophilic, and if they absorb moisture they usually suffer a structural change, such as contraction, and deteriorate, but degradation can be prevented by making them hydrophobic, via a chemical treatment. Aerogels with hydrophobic interiors are less susceptible to degradation than aerogels with only an outer hydrophobic layer, especially if a crack penetrates the surface. Knudsen effect Aerogels may have a thermal conductivity smaller than that of the gas they contain. This is caused by the Knudsen effect, a reduction of thermal conductivity in gases when the size of the cavity encompassing the gas becomes comparable to the mean free path. Effectively, the cavity restricts the movement of the gas particles, decreasing the thermal conductivity in addition to eliminating convection. For example, thermal conductivity of air is about 25 mW·m−1·K−1 at STP and in a large container, but decreases to about 5 mW·m−1·K−1 in a pore 30 nanometers in diameter. Structure Aerogel structure results from a sol-gel polymerization, which is when monomers (simple molecules) react with other monomers to form a sol or a substance that consists of bonded, cross-linked macromolecules with deposits of liquid solution among them. When the material is critically heated, the liquid evaporates and the bonded, cross-linked macromolecule frame is left behind. The result of the polymerization and critical heating is the creation of a material that has a porous strong structure classified